USE OF MERCURY POROSIMETRY AND NITROGEN ADSORPTION IN CHARACTERISATION OF THE PORE STRUCTURE OF MANNITOL
USE OF MERCURY POROSIMETRY AND NITROGEN ADSORPTION IN CHARACTERISATION OF THE PORE STRUCTURE OF MANNITOL
Pharmaceutical Technology Division Department of Pharmacy University of Helsinki Finland USE OF MERCURY POROSIMETRY AND NITROGEN ADSORPTION IN CHARACTERISATION OF THE PORE STRUCTURE OF MANNITOL AND MICROCRYSTALLINE CELLULOSE POWDERS, GRANULES AND TABLETS Sari Westermarck Academic Dissertation To be presented, with the permission of the Faculty of Science of the University of Helsinki, for public criticism in Auditorium XII on November 8, 2000 at 12 noon Helsinki 2000
ISBN 952-91-2534-8 (printed) ISBN 952-91-2535-6 (pdf) ISBN 952-91-2536-4 (html) Helsinki 2000 Yliopistopaino
To Risto, Werner, Roy and Henrik
CONTENTS 1 INTRODUCTION . 1 2 THEORY . 2 2.1 Porosity . . 2 2.2 Mercury porosimetry . . 2 2.2.1 Mercury porosimetry procedure . . 2 2.2.2 Washburn equation . . 3 2.2.3 Total pore volume and total pore surface area . . 4 2.2.4 Mean and median pore diameter . . 4 2.2.5 Volume pore size distribution . . 5 2.2.6 Use of mercury porosimetry in pharmaceutical powder technology . . 5 2.2.7 Advantages and limitations of mercury porosimetry . . 6 2.3 Nitrogen gas adsorption method . . 7 2.3.1 Total pore volume and volume pore size distribution .
. 7 2.3.2 Specific surface area . . 9 2.3.3 Use of nitrogen adsorption in pharmaceutical powder technology . . 9 2.3.4 Advantages and limitations of nitrogen gas adsorption . . 9 2.3.5 Comparison of nitrogen adsorption and mercury porosimetry methods . . 10 2.4 Water vapour adsorption . . 11 2.4.1 Adsorption of water on the surface of a solid sample . . 11 2.4.2 Behaviour of water in the pores . . 11 2.5 Mannitol . . 12 2.5.1 Characteristics of mannitol and its behaviour in wet granulation and tableting . . 12 2.6 Microcrystalline cellulose . . 13 2.6.1 Characteristics of microcrystalline cellulose and its mechanism of swelling .
. 13 2.6.2 Behaviour of microcrystalline cellulose in wet granulation and tableting . . 16 3 AIMS OF THE STUDY . . 18 4 EXPERIMENTAL . . 19 4.1 Materials (I-V . . 19 4.2 Characterisation of powders . . 19 4.2.1 Particle size, appearance, water adsorption isotherms and moisture content (I . . 19 4.2.2 Pore structure obtained by mercury porosimetry (I-III . . 19 4.2.3 Pore structure and specific surface area obtained by nitrogen adsorption (I–III . . 20 4.3 Granulation (I-V . . 20 4.4 Characterisation of granules . . 21 4.4.1 Particle size, appearance, water adsorption isotherms and moisture content (I .
. 21 4.4.2 Pore structure obtained by mercury porosimetry (I-III . . 21 4.4.3 Pore structure and specific surface area obtained by nitrogen adsorption (I-III . . 21 4.5 Characterisation of powder and granule masses before tableting . . 21 4.6 Tableting (II-V . . 21
4.7 Characterisation of tablets . . 22 4.7.1 Breaking force and moisture content (II-V . . 22 4.7.2 Porosity based on tablet dimensions (II-III . . 22 4.7.3 Pore structure obtained by mercury porosimetry (II-V . . 22 4.7.4 Pore structure and specific surface area obtained by nitrogen adsorption (II-III . . 22 4.8 Statistical analysis (I, IV-V . . 23 5 RESULTS AND DISCUSSION . . 24 5.1 Effect of pretreatment by vacuum drying or by storage in moisture conditions on the result of mercury porosimetry analysis, and the role of moisture in the structure of the samples during mercury porosimetry .
. 24 5.1.1 Non-hygroscopic mannitol and hygroscopic microcrystalline cellulose powder (I . . 24 5.1.2 Non-hygroscopic mannitol and hygroscopic microcrystalline cellulose granules (I . . 24 5.1.3 Tablet samples (IV, V . . 25 5.2 Effect of scanning speed on the result of mercury porosimetry analysis . . 29 5.2.1 Powder samples (I . . 29 5.2.2 Granule samples (I . . 29 5.2.3 Tablets (IV, V . . 30 5.3 Effect of wet granulation and tableting on the pore structure of mannitol and micro- crystalline cellulose . . 32 5.3.1 Mannitol (II . . 32 5.3.2 Microcrystalline cellulose (III . . 35 5.4 Comparison of mercury porosimetry and nitrogen adsorption methods in determination of pore structure .
. 40 5.4.1 Powders (II, III . . 40 5.4.2 Granules (II . . 40 5.4.3 Tablets (II, III . . 41 5.4.4 Surface area results (II, III . . 42 6 CONCLUSIONS . . 43 REFERENCES . . 45 ORIGINAL PUBLICATIONS
ACKNOWLEDGEMENTS This work was carried out in 1993 – 2000 at the Pharmaceutical Technology Division, Department of Pharmacy, University of Helsinki and at the Department of Physical Pharmacy, Orion Corporation, Orion Pharma. I express my deepest gratitude to Docent Anne Juppo, Ph. D. (Pharm.) for suggesting me the topic of this study and showing me how to use physical pharmacy as a tool in pharmaceutical technology. I also express my gratitude to Professor Jouko Yliruusi, Ph. D. (Pharm.), M. Sc. (Phys.). Their excellent examples as persons in connecting science and practise in pharmaceutical industry have led me through these years and made this work possible and interesting for me.
I am grateful to Dr. Åsa Adolfsson Ph. D. (Pharm.) and Professor Kari Heiskanen D.Sc. (Tech.), the official referees of this thesis for their constructive comments and suggestions concerning the manuscript. I owe my sincere thanks to Vice President Marja Ritala, Ph. D. (Pharm.), Head of Department Mervi Niskanen, Ph. D. (Pharm.) and Docent Veli Pekka Tanninen, Ph. D. (Physics) at Orion Pharma for the possibility to continue my studies and for placing the facilities of the laboratories at my disposal.
My thanks are also due to my co-authors Katri Koiranen, M. Sc. (Pharm.) and Lasse Kervinen M.
Sc. (Phys.) for their collaboration. The personnel of the Department of Physical Pharmacy/Laboratory of Physics and Information Services Department at Orion Pharma are warmly thanked for their collaboration. I thank Harri Salonen B.A., for revising the language of the English manuscript of this thesis. I am also very grateful to my parents, Ulla and Urho, for their encouragement during these years. Financial support from the Finnish Cultural Foundation, Elli Turunen Foundation, is acknowledged.
Espoo, October 2000
ABSTRACT USE OF MERCURY POROSIMETRY AND NITROGEN ADSORPTION IN CHARACTERISATION OF THE PORE STRUCTURE OF MANNITOL AND MICROCRYSTALLINE CELLULOSE POWDERS, GRANULES AND TABLETS Sari Westermarck, 2000, University of Helsinki (FIN), pp. 50. ISBN952-91-2534-8 The effects of pretreatment and scanning speed of mercury porosimetry on the mercury porosimetry results of non-hygroscopic mannitol and hygroscopic microcrystalline cellulose powder, granule and tablet samples were studied. Behaviour of water in the structure of these samples during mercury porosimetry was evaluated.
The effect of granulation and tableting on the pore structure of mannitol and microcrystalline cellulose was investigated. Furthermore, mercury porosimetry and nitrogen adsorption methods were compared.
Granules were manufactured by wet granulation with a high-shear mixer. Tablets were prepared both by direct compression and from granules with an instrumented rotary press using three compression pressures. Porosity parameters were determined with mercury porosimetry and nitrogen adsorption. Pretreatment has an effect on mercury porosimetry results of non-hygroscopic mannitol and hygroscopic microcrystalline cellulose samples. Water affects with different mechanisms the results of samples of different physical structures, i.e. powder, granule and tablet samples. Water surprisingly increases the volume of the smallest pores of both mannitol and microcrystalline cellulose granules in high-pressure mercury porosimetry.
Similarly, water increases the volume of the smallest pores of microcrystalline cellulose tablets compressed from granules with the highest compression pressure used in the study. Water condenses into the smallest pores of microcrystalline cellulose tablets manufactured by direct compression, hinders the intrusion of mercury and decreases the volume of the smallest determined pores. Water settles into the structure of mannitol and microcrystalline cellulose tablets in the pore diameter range of 50 – 2000 nm and 500 – 2000 nm, respectively. Maximum of the volume pore size distribution at this pore size range shifts towards larger pores with increasing moisture.
Proper pretreatment and determination of water content of the samples before mercury porosimetry measurement is important. Due to low scanning speeds used in the measurements, scanning speed does not have an effect on the result of low-pressure porosimetry analysis. Total pore volume determined with high-pressure porosimetry is unaffected by scanning speed, too. However, other porosity parameters determined with high-pressure porosimetry were influenced when different scanning speeds were used in determinations. The smallest pores of the samples were not accurately determined with fast scanning.
In tablet samples, scanning speed affected the pore structure determinations even in the larger pore size range. Therefore, slow scanning speed in the measurements is preferable.
Wet granulation increased the compactibility of mannitol, but decreased that of microcrystalline cellulose. Mannitol granules had a porous structure, whereas microcrystalline cellulose granules were hard, dense and non-porous. Mannitol powder and granules deformed by fragmentation and plastic deformation under compression. Microcrystalline cellulose powder deformed plastically, and the structure of hard granules was destroyed when compressed with the highest compression pressure. The pore structure obtained with mercury porosimetry describes the behaviour of powder and granules and the voids between them in granulation and compression.
Nitrogen adsorption emphasizes the changes in the intraparticular structure of the particles during compression. Due to the low porosity of pharmaceutical samples and the different measurement ranges of these methods, total pore volume, specific surface area and intensities of volume pore size distributions obtained with these two methods are not equivalent. Pores of mannitol samples are detected at the same pore size range with both methods. However, microcrystalline cellulose samples may be deformed during mercury porosimetry measurement, because the pores are not determined at the same pore size range as with nitrogen adsorption.
Volume pore size distribution is a useful parameter showing where the changes in the structures of the samples occur during processing. Specific surface area obtained with nitrogen adsorption describes well the behaviour of pharmaceutical materials during compression. Together mercury porosimetry and nitrogen adsorption describe well the behaviour of materials in pharmaceutical processes.
LIST OF ORIGINAL PUBLICATIONS This thesis is based on the following original papers, which are referred to in the text by the Roman numerals I – V. I Westermarck, S., Juppo, A.M., Koiranen, K. and Yliruusi, J., 1998. Mercury porosimetry of pharmaceutical powders and granules. J. Porous Mater. 5, 77-86. II Westermarck, S., Juppo, A.M., Kervinen, L. and Yliruusi, J., 1998. Pore structure and surface area of mannitol powder, granules and tablets determined with mercury porosimetry and nitrogen adsorption. Eur. J. Pharm. Biopharm. 46, 61-68. III Westermarck, S., Juppo, A.M., Kervinen, L. and Yliruusi, J., 1999.
Microcrystalline cellulose and its microstructure in pharmaceutical processing. Eur. J. Pharm. Biopharm. 48, 199 – 206.
IV Westermarck, S., Juppo, A.M. and Yliruusi, J., 2000. Mercury porosimetry of mannitol tablets: effect of scanning speed and moisture. Pharm. Dev. Technol. 5 (2), 181 – 188. V Westermarck, S., 2000. Mercury porosimetry of microcrystalline cellulose tablets: effect of scanning speed and moisture. Eur. J. Pharm. Biopharm. 50, 319 – 325.
ABBREVIATIONS A area am cross-sectional area of molecule c BET constant d diameter dmean mean pore diameter dmedian median pore diameter Dv(d) volume pore size distribution G Gibbs free energy L length m weight n number of moles na Avogadro constant p pressure pGAS gas pressure above ambient p0 saturated vapor pressure r radius R gas constant S total pore surface area SBET specific surface area T absolute temperature V volume Vc condensed volume VL molar volume Vm volume of monolayer VTOT total pore volume W work ε porosity γ surface tension γLV liquid-vapor interaction γSL solid-liquid interaction γSV solid-vapor interaction ρb bulk density ρh true density θ contact angle